(3) MEMÒRIA PRESENTADA PER ASPIRAR AL GRAU DE DOCTOR PER SARA GÓMEZ DE PEDRO:. SARA GÓMEZ DE PEDRO VIST I PLAU:. MARIA DEL MAR PUYOL BOSCH. JULIÁN ALONSO CHAMARRO. Professor Lector (Ajudant Doctor). Catedràtic de Química Analítica. BELLATERRA (CERDANYOLA DEL VALLÈS), 23 DE JULIOL DE 2014.
(5) The present dissertation has been carried out thanks to the following financial support: Nanotecnologías en Biomedicina (CONSOLIDER INGENIO2010-CSD2006-12). Ministerio de Educación y Ciencia.. Construcción de Microanalizadores de Parámetros de Interés Medioambiental Mediante el Uso de Tecnologías IC y LTCC (CIT-310200-2007-29). Ministerio de Educación y Ciencia.. Nuevas plataformas de microfluidica para la miniaturizacion de sistemas (bio)analiticos integrados e intensificacion de procesos de produccion de nanomateriales (CTQ2009-12128). Ministerio de Educación y Ciencia.. Miniaturizacion, integracion y paralelizacion de ensayos quimicos y biologicos mediante nuevas plataformas de microfluídica (CTQ2012-36165). Ministerio de Educación y Ciencia co-funded by FEDER. Grup de Sensors i Biosensors, Grupo de investigación consolidado (2009SGR0323). Generalitat de Catalunya.. Grup de Sensors i Biosensors Unitat de Química Analítica Departament de Química Universitat Autònoma de Barcelona Edifici Cn 08193 Bellaterra, España Telf. 0034 581 2533 Fax. 0034.
(7) The described work result in the following publications: Sara Gomez de Pedro, Mar Puyol, Julián Alonso, Continuous flow synthesis of nanoparticles using ceramic microfluidic devices, Nanotechnology, 2010, 21, 41.. Sara Gomez-de Pedro, Mar Puyol, David Izquierdo, Iñigo Salinas, Jesús Martínez de la Fuente, Julián Alonso-Chamarro, A ceramic microreactor for the synthesis of water soluble CdS and CdS/ZnS nanocrystals with on-line optical characterization, Nanoscale, 2012, 4(4), 1328-1335.. Sara Gómez-de Pedro, Cynthia S. Martínez-Cisneros, Mar Puyol and Julián AlonsoChamarro, Microreactor with integrated temperature control for the synthesis of CdSe nano crystals, Lab on a Chip, 2012, 12 (11), 1979-1986.. Cynthia S. Martínez-Cisneros, Sara Gómez-de Pedro, J. García-García, Mar Puyol and Julián Alonso-Chamarro, Design, fabrication and characterization of microreactors for high temperature syntheses, Chemical Engineering Journal, 2012, 211-212, 432-441.. Sara Gómez-de Pedro, Daniela Lopes, Sergey Miltsov, David Izquierdo, Julian AlonsoChamarro and Mar Puyol, Optical microfluidic system based on ionophore modified gold nanoparticles for the continuous monitoring of mercuric ion, Sensors and Actuators B, 2014, 194, 19-26.. Sara Gómez, Alfonso Salinas-Castillo, Maria Ariza-Avidad, Ajejandro Lapresta, Cristina Sánchez-González, Cynthia Susana Martínez-Cisneros, Mar Puyol, Luis Fermin Capitan-Vallvey and Julián Alonso, Microsystem-assisted synthesis of carbon dots with fluorescent and colorimetric properties for pH detection, Nanoscale, 2014, 6, 6018-6024.. Sara Gómez-de Pedro, Miguel Berenguel-Alonso, Pedro Couceiro, Julián AlonsoChamarro, Mar Puyol, Automatic Microfluidic System to Perform a Multi-Step Magneto-Biochemical Assay. (Draft in progress). Other publications related to this work and in collaboration with other studies are: Sergey Miltsov, Vladimir Karavan, Vadim Boyarsky, Sara Gómez-de Pedro, Julian Alonso-Chamarro and Mar Puyol, New acyclic Pd-diaminocarbene catalyst for Suzuki arylation of meso-chlorosubstituted tricarboindocyanine dyes, Tetrahedron Letters, 2012, 54(10), 1202-1204. Pedro Couceiro, Sara Gómez-de Pedro and Julián Alonso-Chamarro, All-ceramic analytical microsystems with monolithically integrated optical detection microflow cells. Microfluidics and Nanofluidics. Accepted manuscript..
(8) Sergey Miltsov, Vladimir Karavan, Mikhail Goikhman, Irina Podeshvo, Sara Gómez-de Pedro, Mar Puyol and Julian Alonso-Chamarro, Synthesis of bis-aminosubstituted indocyanine dyes for their use in polymeric compositions. Dyes and Pigments, 2014, 109, 34-41.. Oriol Ymbern, Miguel Berenguel-Alonso, Antonio Calvo-López, Sara Gómez-de Pedro and Julián Alonso-Chamarro, Microfluidic cartridge reader for optical measurements in continuous flow and batch procedures. Analytical Chemistry. Submitted to the journal. Sara Gómez-de Pedro, Sergey Miltsov, Julian Alonso-Chamarro and Mar Puyol, Spectroscopic characterization of new bis-acetylamino and bis-amino substituted cyanine dyes for their use in analytical applications. (Draft in progress).. Sergey Miltsov, Vladimir Karavan, Alexey Mindich, Mar Puyol, Sara Gomez, Julian Alonso, Synthesis and spectroscopic characterization of water-soluble ketocyanine dyes with cyclic fragments in the polymethine chain for their use in optical sensors. (Draft in progress)..
(11) TABLE OF CONTENTS.
(13) 1 INTRODUCTION 1.1 MINIATURIZATION OF ANALYTICAL SYSTEMS .......................... 1.1.1 Microfluidic Platforms 1.1.2 Integrating Operations of the Analytical Process in Microsystems 184.108.40.206 Sample Pre-treatment 220.127.116.11 Detection Systems 1.1.3 Materials and Microfabrication Methods 18.104.22.168 Silicon Technology 22.214.171.124 Polymers Technology Cyclic Olefin Copolymer 126.96.36.199 LTCC Technology 1.2 NANOTECHNOLOGY AND ANALYTICAL CHEMISTRY ................ 1.2.1 Nanoparticles and its Role in Analytical Chemistry 1.2.2 Nanoparticles for Colorimetric Assays 188.8.131.52 Silver Nanoparticles 184.108.40.206 Gold Nanoparticles 1.2.3 Nanoparticles for Fluorimetric Assays 220.127.116.11 Quantum Dots 18.104.22.168 Carbon Dots 1.2.4 The Case of Biosensors 1.3 SYNTHESIS AND CHARACTERIZATION OF NANOPARTICLES .... 1.3.1 Synthesis of Nanoparticles 22.214.171.124 Metallic Nanoparticles Silver Nanoparticles Gold Nanoparticles 126.96.36.199 Quantum Dots Chemical Precipitation (Aqueous Media Approaches) Thermal Decomposition (Organic Media Approaches) Nanocrystals Solubilization Core-shell Quantum Dots 188.8.131.52 Carbon Dots 1.3.2 Characterization of Nanoparticles 184.108.40.206 Microscopic techniques Transmission Electron Microscopy Atomic Force Microscopy Confocal Laser Scanning Microscopy 220.127.116.11 Spectroscopic Techniques UV-Vis Spectroscopy Fluorescence Spectroscopy Atomic Emission Spectroscopy Energy-Dispersive X-Ray Spectroscopy. 1 4 4 6 6 7 9 9 10 11 12 14 18 23 25 26 28 29 33 38 43 44 48 48 49 50 50 51 53 54 54 55 56 56 57 57 58 58 59 60 61.
(14) Selected Area Electron Diffraction Dynamic Light Scattering 18.104.22.168 Other techniques Gravimetric Analysis Zeta Potential 1.4 MICROSYSTEMS AND NANOTECHNOLOGY ............................... 1.4.1 Microsystems based on Nanoparticles 1.4.2 Microreactors for the Synthesis of Nanoparticles. 62 62 63 63 64 65 65 70. 2 OBJECTIVES. 79. 3 FABRICATION PROCEDURES. 83. 3.1 LOW TEMPERATURE COFIRED CERAMICS FABRICATION PROCEDURE LTCC ............................................................................ 3.1.1 Design 3.1.2 Layers Machining 3.1.3 Screen-Printing of Conductive Pastes 3.1.4 Lamination 3.1.5 Sintering process 3.1.6 Inspection of the Fabrication Process 3.2 CYCLIC OLEFIN COPOLYMER FABRICATION PROCEDURE ........ 3.2.1 Design 3.2.2 Layers Machining 3.2.3 Lamination 3.2.4 Inspection of the Fabrication Process 3.3 CONSTRUCTED MICROFLUIDIC PLATFORMS AND INTEGRATION OF OTHER COMPONENTS ....................................... 4 MICROREACTORS FOR THE SYNTHESIS OF METALLIC NANOPARTICLES 4.1 MICROREACTOR FOR THE SYNTHESIS OF SILVER NANOPARTICLES (MR1) .................................................................. 4.1.1 Materials, Reagents and Methods 4.1.2 Experimental Set-up 4.1.3 Optimization of the Microfluidic Platform 4.1.4 Optimization of the Chemical and Hydrodynamic Parameters 22.214.171.124 Stabilizing Agent 4.1.5 Conclusions 4.2 MICROFLUIDIC PLATFORM FOR THE SYNTEHSIS OF GOLD NANOPARTICLES (MR2, MR3) ......................................................... 4.2.1 Materials, Reagents and Methods 4.2.2 Experimental Set-up 4.2.3 Optimization of the Microfluidic Platform 4.2.4 Optimization of the Chemical and Hydrodynamic. 83 84 85 86 88 89 90 90 91 91 93 94 94. 99 99 100 101 103 106 109 110 111 112 113 114 116.
(15) Parameters 4.2.5 Stabilizing Agents 4.2.6 Monitorization 4.2.7 Conclusions. 5 MICROREACTORS FOR THE SYNTHESIS OF FLUORESCENT NANOPARTICLES 5.1 MICRORECTORS FOR THE SYNTHESIS OF WATER SOLUBLE CdS AND CdS/ZnS NANOCRYSTALS (MR4, MR5) ............................................................................................... 5.1.1 Materials, Reagents and Methods 5.1.2 Experimental Set-up 5.1.3 CdS Nanocrystals Synthesis 5.1.4 Core-Shell CdS/ZnS Nanocrystals Synthesis 5.1.5 Absorbance and Fluorescence Monitoring 5.1.6 Conclusions 5.2 MICROREACTORS FOR THE SYNTHESIS OF CdSe QUANTUM DOTS (MR6) ....................................................... 5.2.1 Materials, Reagents and Methods 5.2.2 Experimental Set-up 5.2.3 Development of the Thermal Platform 126.96.36.199 Electronics for Temperature Control 5.2.4 Development of the Microfluidic Platform 5.2.5 Characterization of the Thermal and Fluidic Platforms of the Microreactor 188.8.131.52 Thermal Characterization of the Microreactor Modular Configuration Monolithic Configuration 184.108.40.206 Fluidic Characterization of the Microreactor 5.2.6 Synthesis of Nanocrystals 5.2.5 Conclusions 5.3 MICROREACTOR FOR THE SYNTHESIS OF CARBON DOTS (MR7) .................................................................................... 5.3.1 Materials, Reagents and Methods 5.3.2 Experimental Set-up 5.3.3 Development of the Microreactor 5.3.4 Synthesis of Carbon Dots 5.3.5 Conclusions. 6 ANALYTICAL MICROSYSTEMS BASED ON THE USE OF NANOPARTICLES 6.1 MICROSYSTEM FOR MONITORING MERCURIC ION (AMS) ......................................................................................... 6.1.1 Materials, Reagents and Methods 6.1.2 Experimental Set-up. 119 126 128. 131 132 133 134 135 137 140 142 143 144 146 147 153 155 155 156 156 157 158 159 164 165 166 167 168 169 172. 175 176 177 179.
(16) 6.1.3 Development of the Selective Recognition Optical Element 220.127.116.11 Design and Synthesis of the Ionophore 18.104.22.168 Preparation of the Gold Nanoparticles Modified with the Ionophore 6.1.4 Evaluation of the Selective Recognition Optical Element 6.1.5 Microfluidic Platform Design 6.1.6 Evaluation of the Microsystem for the Mercuric Ion Monitoring 6.1.7 Conclusions 6.2 MICROSYSTEM TO PERFORM MULTI-STEP MAGNETOBIOCHEMICAL ASSAYS (BMS) ............................................... 6.2.1 Materials, Reagents and Methods 6.2.2 Experimental Set-up 6.2.3 Functionalization of Magnetic Beads 6.2.4 Development of the Microfluidic Platform 6.2.5 Multi-Step Magneto-Biochemical Assay 22.214.171.124 Description of the Assay Procedure 126.96.36.199 Optimization of the Microsystem for the Multistep DNA Assay 188.8.131.52 Analytical Features of the Microsystem for the Determination of E. coli 6.2.6 Conclusions. 180 181 182 184 186 187 189 190 193 195 196 197 198 199 201 203 204. 7 CONCLUDING REMARKS AND FUTURE PERSPECTIVES. 209. APPENDIX A: CAD DESIGNS. 211. A.1 CAD DESIGN OF MR1 A.2 CAD DESIGN OF MR2 A.3 CAD DESIGN OF MR3 A.4 CAD DESIGN OF MR3 WITH INTEGRATED OPTICAL DETECTION A.5 CAD DESIGN OF MR4 A.6 CAD DESIGN OF MR5 A.7 CAD DESIGN OF MR5MICROREACTOR WITH INTEGRATED OPTICAL DETECTION A.8 CAD DESIGN OF MR6 A.9 CAD DESIGN OF MR7 A.10 CAD DESIGN OF AMS FOR MERCURIC ION MONITORING A.11 CAD DESIGN OF BMS FOR E. COLI DETECTION. APPENDIX B: PUBLICATIONS B.1 Continuous Flow Synthesis of Nanoparticles using Ceramic Microfluidic devices B.2 A Ceramic Microreactor for the Synthesis of Water Soluble CdS and CdS/ZnS Nanocrystals with On-Line. A.1 A.2 A.3 A.4 A.5 A.6 A.7 A.8 A.9 A.10 A.11. 235 B.3 B.5.
(17) Optical Characterization B.3 Microreactor with Integrated Temperature Control for the Synthesis of CdSe Nanocrystals B.4 Design, Fabrication and Characterization of Microreactors for High Temperature Syntheses B.5 Optical Microfluidic System based on Ionophore Modified Gold Nanoparticles for the Continuous Monitoring of Mercuric Ion B.6 Microsystem-Assisted Synthesis of Carbon Dots with Fluorescent and Colorimetric Properties for pH Detection. B.7 B.9 B.11 B.13.
(21) § A, Abs A AA AES AFM Ag NPs AMD AOT Au NPs b BMD c C CAD C-C CCD C-dots/Cdots CE CEC CdO CLPL CNC CNTs COC CTAB DAQ DDT DHLA DLS DNA DWNTs ε EA Escherichia coli EDS E-Field ELISA EPA FRET FTIR FWHM G ∆G GC GSB. Section Absorbance Adenine Atomic Absorption Atomic Emission Spectroscopy Atomic Force Microscopy Silver nanoparticles Analytical microsystem Dioctyl sulfosuccinate Gold nanoparticles Path length Bioanalytical microsystem Concentration Cytosine Computer-Aided Design Carbon-Carbon Charge-Coupled Device Carbon dots Capillary Electrophoresis Capillary Electrochromatography Cadmium oxide Cold and Low Pressure Lamination Computer Numerically Controlled Cabon Nanotubes Cyclic Olefin Copolymer Cetyltrimethylammonium bromide Data Acquisition Card Dodecanethiol Dihygrolipid acid Dynamic Light Scattering DeoxyriboNucleic Acid Double-Wall Nanotubes Molar Absorptivity Elemental Analysis E. coli Energy-Disperse X-Ray Spectroscopy Electromagnetic Field Enzyme-Linked ImmunoSorbent Assay Environmental Protection Agency Fluorescence Resonance Energy Transfer Fourier Transform Infrared Spectroscopy Full Width at Half Maximum Guanine Gibbs free energy Gas Chromatography Group of Sensors and Biosensors.
(22) 2. Acronyms. GTF HOMO HRTEM HTCC I I0 ICP ICP-AES ICP-MS ICP-OES IR LC LED LOC LTCC LUMO MAA MB MCE MEF MEMS MNPs MOSFET MPA MR MSA MUA MUD MWNTs µ-TAS MUA NA POF NMR NPs NT NTC OA ODE OLA ONP ONPG PCB PCR PDMS PEG PID. Grupo de Tecnologías Fotónicas Highest Occupied Molecular Orbital High Resolution Transmission Electron Microscopy High Temperature Co-fired Ceramics Transmitted light intensity Incident light intensity Inductive Coupled Plasma Inductively Coupled Plasma Atomic Emission Spectrometry Inductive Coupled Plasma Mass Spectrometry Inductively Coupled Plasma Optical Emission Spectrometry Infrared Liquid Chromatography Light-emitting diode Lab-on-a-chip Low Temperature Co-fired Ceramic Lowest Unoccupied Molecular Orbital Mercaptoacetic acid Magnetic Bead Microchip Electrophoresis Metal Enhanced Fluorescence Micro Electro Mechanical Systems Metallic Nanoparticles Metal Oxide Semiconductor Field Effect Transistor Mercaptorpopionic acid Microreactor Mercaptosuccinic acid 11-Mercaptoundecanoic acid 11-mercapto-1-undecanol Multi-Wall Nanotubes micro Total Analysis System Mercaptoundecanoic acid Low Numerical Aperture Polymer Optical Fiber Nuclear Magnetic Resonance Nanoparticles 1,8-octanedithiol Negative Temperature Coefficient Oleic acid Octadecene Oleylamine Ortho-nitrophenol Ortho-nitrophenyl-β-galactoside Printed Circuit Board Polymerase Chain Reactions Polydimethylsiloxane Poly(ethylene) glycol Proportional-Integral-Derivative.
(23) Acronyms. PMT PTC PTFE QDs QY, Φ f Rh RTD SAED SEM SPP SPR PSP SWCT TEM Tg TOAB TOP TOPO TP TPP RF SAED SAXS SCC SDS SEM SERS SIMS SPM SPR T TBP TEM Tg TOAB TOP TOPO TPP PVP UAB UCPL UV Vis WHO XRD. Photomultiplier Tube Positive Temperature Coefficient Polytetrafluoroethylene Quantum dots Quantum Yield Rhodamine 6G Resistance Temperature Detector Selected Area Electron Diffraction Scanning Electron Microscopy bis-Sulphonated triphenylphosphine Surface Plasmon Resonance Pseudo-stationary Phase Single-Wall Nanotubes Transmission Electron Microscopy Glass-transition temperature Tetraoctylammonium bromide Trioctylphosphine Trioctylphosphine oxide Tiopronin, N-(2-Mercaptopropionyl) glycine Triphenylphosphine Radio Frequency Selected Area Electron Diffration Small Angle X-ray Scattering Signal Conditioning Circuit Sodium dodecylsulfonate Scanning Electron Microscopy Surface Enhancement Raman Scattering Secondary Ion Mass Spectrsocopy Scanning Probe Microscopy Surface Plasmon Resonance Thymine Tributylphosphine Transmission Electron Microscopy Glass Transition Temperature Tetraoctylammonium bromide Trioctylphosphine Trioctylphosphine oxide Triphenylphosphine Poly(vinylpyrrolidone) Universitat Autònoma de Barcelona Up-Conversion Photoluminiscence Ultraviolet Visible World Health Organization X-Ray Diffraction. 3.
(24) 4. Acronyms.
(25) SUMMARY. Image from Lab-on-a-chip.gene-quantification.info.
(27) D. emand for new automated analytical procedures and instrumentation for the continuous monitoring of (bio)chemical parameters, such as those affecting water quality, gathers special importance due to the significant consequences that the use or the consumption of (bio)chemically contaminated water might have. µ- Total Analysis Systems or Lab-On-a-Chip devices are increasingly employed with this purpose owing to the high integration and automation of these devices that allow, through miniaturization, the possibility of performing in situ measurements. Besides, the use of nanoparticles with analytical purposes has demonstrated to improve the sensitivity and detection limits of optical methods. Within this general context, the present work is focused on the development of automated analytical microsystems to perform colorimetric or fluorimetric analyses, based on the use of nanoparticles as optical labels, for the rapid detection of water pollutants or organisms, such as heavy metals or bacteria. However, the use of nanoparticles with identical physical characteristics is a must in order to obtain reliable and reproducible analytical measures. Therefore, the first part of this work is addressed to the development of microreactors for the synthesis of metallic, semiconductor and carbon nanoparticles. Seven different ceramic microreactors are developed, in which the influence of the design (dimensions and configuration of the channels) and the hydrodynamic (flow rates and dosage volumes) parameters have been studied. Moreover, a miniaturized optical detection system has been implemented for the in-line monitoring of the synthesis; and a thermal module has been also developed to reach and accurately control temperatures up to 300 ºC for when required. It is important to highlight that all prototypes operate automatically, which simplifies the syntheses and improves the reproducibility of the obtained nanoparticles. The second part focuses on the development of analytical microsystems based on the use of the nanoparticles previously synthesized for water quality analysis. Two different prototypes have been constructed and tested. The first described allows the monitoring of mercuric ion in water. The system is based on the selective recognition of the analyte by an ionophore (a thiourea derivative), attached onto gold nanoparticles surface. The metal-ionophore interaction generates a change on the surface plasmon resonance band of the nanoparticles, resulting in a quantifiable optical signal, which is in-line registered by a miniaturized optical detection system integrated in the microfluidic platform. Once optimized, the device is capable to automatically detect up to 11 ppb of mercuric ion. Finally, and as a first approximation to the use of fluorescent nanoparticles within microsystems, a prototype for the determination of Escherichia coli in water has been developed, which uses the β-galactosidase enzyme as label. This change responds to the necessity of improving the miniaturized optical system (while maintaining its portability and.
(28) Summary. low cost) due to the low sensitivity observed when fluorescent nanoparticles were used as labels, which at the moment is not feasible. An oligonucleotide sandwich assay is performed in the microfluidic system based on the use of a specific oligonucleotide of the pathogen as target. On the other hand, magnetic beads are employed as substrate support of the assay, which allow simplifying and improving the different steps of the procedure, while the enzyme used as probe label generates a coloured product (o-nitrophenol) with the addition of the substrate, which is registered through the miniaturized optical system implemented. Once optimized, the device can detect up to 1 ppb of the target oligonucleotide in only 20 minutes. The presented results demonstrate the great potential of automated analytical microsystems based on the use of nanoparticles for the monitoring of water quality. Similarly, the suitability of microreactors for the synthesis of nanoparticles has been well proved..
(29) E. l desarrollo de nuevos procedimientos analíticos e instrumentación automáticos para la monitorización de parámetros (bio)químicos, tales como los que afectan a la calidad del agua, es de especial importancia debido a las graves consecuencias que puede tener el uso o consumo de un agua (bio)químicamente contaminada. Los microsistemas de análisis total o dispositivos Lab-On-a-Chip son cada vez más empleados con este propósito debido a la gran integración y automatización que ofrecen estos dispositivos, a través de la miniaturización, y a la posibilidad de realizar medidas in situ. Por otro lado, el uso de nanopartículas con fines analíticos ha demostrado mejorar la sensibilidad y límites de detección de métodos ópticos. Así, esta tesis se centra en el desarrollo de microsistemas analíticos automatizados que llevan a cabo análisis colorimétricos o fluorimétricos, basados en el uso de nanopartículas como marcadores ópticos, para la rápida detección de analitos o microorganismos de contaminación hídrica, tales como metales pesados o bacterias. Sin embargo, es necesario utilizar nanopartículas con idénticas características físicas para obtener medidas analíticas fiables. Así, la primera parte de este trabajo abarca el desarrollo de microreactores para la síntesis controlada y reproducible de nanopartículas metálicas, semiconductoras y de carbono. Se muestran un total de siete microreactores, en los que se ha realizado un estudio de los parámetros de diseño e hidrodinámicos. Además, se ha implementado un sistema de detección óptica miniaturizado para la monitorización en línea de la síntesis; y se ha desarrollado un módulo térmico que permite alcanzar y controlar temperaturas de hasta 300 ºC para aquellas reacciones que lo requieran. Es de destacar que los microsistemas trabajan de forma automática y programable, lo cual simplifica el procedimiento de síntesis y mejora la reproducibilidad de las nanopartículas obtenidas. La segunda parte del trabajo se centra en el desarrollo de microsistemas analíticos basados en la utilización de las nanopartículas sintetizadas para el análisis de algún parámetro de la calidad del agua. Se han construido y evaluado dos prototipos. El primero de ellos está diseñado para la monitorización de ión mercurio en agua. El sistema se basa en el reconocimiento selectivo del analito mediante un ionóforo (un derivado de la tiourea) unido a la superficie de nanopartículas de oro. La interacción metal-ionóforo provoca un cambio en la banda del plasmón superficial de las nanopartículas, generando una señal óptica cuantificable que se registra en línea mediante un sistema óptico integrado en la plataforma microfluídica. Una vez optimizado, el dispositivo es capaz de detectar hasta 11 ppb de mercurio(II). Finalmente, y como primera aproximación al uso de nanopartículas fluorescentes en microsistemas, se ha desarrollado un prototipo para la determinación de Escherichia coli en agua utilizando como marcador la enzima β-galactosidasa. Este cambio responde a la necesidad de mejorar el sistema óptico miniaturizado (manteniendo su portabilidad y bajo coste), debido a la baja sensibilidad observada cuando nanopartículas.
(30) Resumen. fluorescentes fueron usadas como marcadores. El dispositivo desarrollado lleva a cabo un ensayo tipo sándwich de oligonucleótidos, dónde se emplea como sonda diana un oligonucleótido específico del patógeno. El uso de micropartículas magnéticas como sustrato soporte del ensayo permite simplificar y mejorar las distintas etapas del análisis, mientras que el enzima usado como marcador de la sonda de reconocimiento genera un producto coloreado al añadir el sustrato, registrado mediante el sistema óptico miniaturizado implementado. Tras su optimización, es posible detectar 1 ppb de la sonda diana en 20 minutos. Los resultados presentados en este trabajo muestran el gran potencial de los microsistemas analíticos automatizados basados en el uso de nanopartículas para monitorizar la calidad del agua. Se ha demostrado también la idoneidad de los microreactores para la síntesis de nanopartículas..
(31) 1. INTRODUCTION Contents 1.1 Miniaturization of Analytical Systems ........................................................... 1.1.1 Microfluidic Platforms 1.1.2 Integrating Operations of the Analytical Process in Microsystems 1.1.3 Materials and Microfabrication Methods 1.2 Nanotechnology and Analytical Chemistry ................................................... 1.2.1 Nanoparticles and its role in Analytical Chemistry 1.2.2 Nanoparticles for Colorimetric Assays 1.2.3 Nanoparticles for Fluorimetric Assays 1.2.4 The case of Biosensors 1.3 Synthesis and Characterization of Nanoparticles ....................................... 1.3.1 Synthesis of Nanoparticles 1.3.2 Characterization of Nanoparticles 1.4 Microsystems and Nanotechnology ............................................................... 1.4.1 Microsystems based on Nanoparticles 1.4.2 Microreactors for the Synthesis of Nanoparticles. Image from Lab-on-a-chip journal. 4 4 6 9 14 18 23 28 38 43 44 55 65 65 70.
(33) he constant demand to obtain real time information and the current strict regulations for environment, food and, generally, the quality control of products, make necessary the improvement of analytical instrumentation. Specifically, water quality determination gathers special importance due to the consequences that may have the use or consumption of contaminated water. For instance, the drinking of water which contain elevated concentrations of heavy metals can lead to the development of neurological, reproductive or cardiovascular diseases, among other disorders. On the other hand, the presence of viruses or pathogens can produce diarrhoea diseases, which can generate even to the death of the patient, when this water is used for its consumption or even only employed for recreational purposes. Therefore, the development of efficient and portable analysis systems for water quality determination is of special interest, since the classical methods employed are time-consuming and require qualified personnel, among other minor inconveniences. As a result, a great interest on this matter has arisen and huge efforts have been done in recent years to develop robust and efficient analytical instrumentation, capable to perform simple, rapid and reproducible analyses. 1. T. For this purpose, the so called Total Analysis Systems (TAS) appeared with the aim of simplifying and automating the analytical process, namely sampling, sample transport, separation, reaction, transduction and signal acquisition. These systems endow connectivity and automation to the different steps of the analytical process, minimizing the operator intervention. In this way, both the costs and the analysis time of the whole process can be reduced as well as possible mistakes due to human manipulation are avoid. However, even these systems present some limitations, such as reduced portability and high reagents consumption. Miniaturization and integration seem to overcome these drawbacks, thus emerging the well-known micro-Total Analysis Systems (μ-TAS) or Lab-on-a-Chip (LOC). 2-3 Their reduced size and weight makes possible to minimize the energy consumption, making feasible to perform in situ measurements. Moreover, by volume miniaturization, the amount of required reagents and therefore also the generation of wastes are reduced, making these systems greener than the conventional ones. Furthermore, they can determine different components of a sample in the same analysis when multiplexing approaches are used. All this contributes to minimize the total cost of the analysis, Alegret, S.; in: Integrated Analytical Systems, Elsevier, Amsterdam, 2003, 1-36. Manz, A.; Graber, N.; Widmer, H.M.; Sens. Actuators, B, 1990, 1, 244. 3 Van den Berg, A.; Bergveld, P.; Lab Chip, 2006, 6, 1266. 1 2.
(34) 2. 1 Introduction. allowing the development of customized systems for personal in situ diagnosis (point-of-care diagnosis) or the direct on-site monitoring of environmental parameters. Besides miniaturization and automation, analytical instrumentation can also take advantage of the exceptional physicochemical properties of nanostructured materials in order to enhance the sensitivity, selectivity, specificity and rapidity of analytical methods by using simple strategies. 4 Nanomaterials are characterized for their large surface area-to-volume ratio, which have demonstrated great potential in all analytical separation techniques, by improving the selectivity, stability and efficiency of the separation. In the same manner, this property is specially interesting when nanomaterials are used as a substrate support for sensing schemes, since multiple molecules can be attached to each nanostructure, which can simplify the assay design and increase sensitivity. 5 Nanomaterials offer the possibility of detecting or manipulating atoms and molecules, such as when used in Surface-Enhanced Raman Spectroscopy (SERS) applications, and have great potential in the development of miniaturized analytical systems, when they are intended to be used for detection purposes. In concrete, the use of as well the electrochemical as the optical properties of some nanoparticles is of special interest, since they have shown enhanced sensitivity and low detection limits compared with some conventional analytical methods. 6 Moreover, the use of metallic or fluorescent nanoparticles as optical detection labels can provides some advantages regarding the use of dyes or fluorophores, such as higher photostability and quantum yields. 7 These materials have also given rise to the development of new types of analytical tools, such as bioimaging, which is very interesting and useful in medical and biochemical applications. 8 The present thesis is addressed to achieve improved analytical instrumentation taking advantage from miniaturization and automation of analysis systems and also from the use of nanomaterials as optical labels to perform colorimetric and fluorimetric determinations. For this purpose, the use of nanomaterials with the same physicochemical properties is essential in order to obtain confident and reproducible results. As it is well known, properties of nanostructured materials, and more concretely nanoparticles, are directly related to their composition, size and morphology, which depend on the followed synthetic procedure, and some related variables, such as the temperature reaction and the molar relationship of reagents.7 Conventional synthetic methods are the most employed procedures for 4. Zhang, X., Guo, Q., Cui, D., 2009. Sensors 9, 1033-1053. Kumar, C.S.S.R., 2007. Nanomaterials for biosensors. Vch Verlagsgesellschaft Mbh. 6 Valcárcel, M.; Simonet, B.M.; Anal. Bioanal Chem., 2011, 399, 1. 7 Cao, G.; Wang, Y.; in: Nanostructures and Nanomaterials. Synthesis, Properties, and Applications; World Scientific Publishing Co. Pte. Ltd. 2on edition, 2011. 8 Wu, C.-S.; Liu, F.-K.; Ko, F.-H.; Anal. Bioanal Chem., 2011, 399, 103. 5.
(35) 1 Introduction. 3. nanomaterials synthesis because a high quantity of product is obtained. However, they are usually time-consuming and limited in some aspects, including a poor control of the reagents concentration in the whole of the solution, and the difficulty of managing the local temperature. As a consequence, heterogeneous products are often obtained within a batch synthesis or even more worse between different batches. Process intensification, which appeared as a strategy for reducing the size of chemical plants so as to reach a given production objective, can help in this issue. It is focused on the development of novel devices to improve a manufacturing process, decreasing the required equipment or their size, energy consumption, or waste production. 9 These strategies are directly related with miniaturization and microfluidics. The main idea in the field of synthesis is to take advantage of the large surface area-to-volume ratios within microchannel structures to accelerate heat and mass transport during a synthetic process. 10 For nanomaterials synthesis in concrete, the rapid changes that can be performed in reaction temperatures and concentrations enables obtaining more uniform products in terms of size and improved reaction yields. In this sense, part of the work presented in this thesis is focused on the development of microfluidic platforms to synthesize homogeneous nanoparticles, which are intended to be exploited in µ-TAS. Figure 1.1 outlines the multidisciplinary nature of the research that has been carried out and the area in which the thesis is framed. Taking this into account, the introduction section of this manuscript is organized in three main parts. The first one is addressed to the miniaturization of analytical systems, including basic concepts about microfluidics and microfabrication techniques. Then, some types of nanomaterials for analytical purposes are described, together with their synthetic methods and the different possible characterization techniques. Finally, the state-of-the-art to µ-TAS based on nanomaterials and also to microreactors for their synthesis of nanomaterials is reported. Materials Microfabrication. µvalves. MINIATURIZATION Electronics µpumps. Fullerenes MICROREACTORS FOR NANOPARTICLES Process intensification. µTAS BASED ON NANOPARTICLES. µfluidic platforms Sample pre-treatments Detection systems. Separation techniques. NANOMATERIALS Quantum dots Metallic nanoparticles SERS. CNTs. (Bio)sensing. Magnetic assay Electrochemical methods. Optical methods ANALYTICAL INSTRUMENTATION. 9. Ramshaw, C.; Proceedings, 1st Intl. Conf. Proc. Intensif. for Chem. Ind., 1995, 18, 1. Stankiewicz, A. I.; Moulijn, J.A.; Chem. Eng. Prog., 2000, January, 22.. 10. Figure 1.1: Scheme of the different related fields for the development of µTAS based on the use of nanomaterials..
(36) 4. 1 Introduction. 1.1 MINIATURIZATION OF ANALYTICAL SYSTEMS Classical chemical analyses are usually performed in laboratories and involve sophisticated and expensive instruments, which require specialized personnel for their operation. Nowadays, an increasing demand of rapid, efficient and exact chemical information exists in order to control the quality of products, to monitor environmental contaminants or the results of a medical care. The development of miniaturized analytical systems becomes a key issue, since these devices are capable to provide in situ qualitative and quantitative information about the composition and nature of a sample in real time at a relative low cost. Besides portability, integration and reduced energy consume, µ-TAS or LOC devices are characterized for their capability to process larger number of samples with limited errors and rapidness due to the lesser manual intervention than conventional instrumentation. Moreover, scaling down increases the surface area to volume ratio, which is very useful for a quick and efficient heat and mass transfer through the microfluidic system, resulting in systems of higher analysis throughput. In addition, miniaturized systems are usually fabricated by means of mass production techniques, which leads to decrease the manufacturing costs and encourage their marketing.. 1.1.1 MICROFLUIDIC PLATFORMS Microfluidic platforms are essential in the development of µ-TAS. They are structures that provide connectivity to the different operations of the chemical analysis such as reagents storage, pre-concentration steps or detection, and, on the other hand, that allow handling of fluids. Transport of fluids, mixing, separating and processing inside the microfluidic platform are performed by means of different fluidic structures by taking advantage of passive fluid control techniques like capillary forces, 11 or using external actuators such as centrifugal forces in rotary drives, 12 or by active (micro) components as (micro)pumps or (micro)valves. 13 Rapid mixing is essential in chemical applications. However, this is difficult to achieve at laminar flows, where mass transport is mainly done by diffusion. Reynolds number, which quantifies the relative importance of the inertial and viscous forces, is the parameter normally used to characterize the different flow regimes, such as laminar or turbulent flows. The first is usually the dominant flow regime in microfluidics, which is characterized by a slow movement of the liquid Lynn, N. S.; Dandy, D.S.; Lab Chip, 2009, 9(23), 3422. Ducrée, J.; Haeberle, S.; Lutz, S.; Pausch, S.; von Stetten, F.; Zengerle, R.; J. Micromech. Microeng., 2007, 17, S103. 13 Gravesen, P.; Branebjerg, J.; Jensen, O.S.; J. Micromech. Microeng., 1993, 3, 168. 11 12.
(37) 1 Introduction. (low Reynolds numbers). The second is dominated by inertial forces and it is defined by flow instabilities as vortices (high Reynolds numbers). 14 The incorporation of passive or active mixers into the microfluidic platform plays major importance, since these structures enhance the grade of reagents mixture by generating turbulent regimes. 15. 5. Figure 1.2: Most common passive micromixers. A) Basic T-shape mixer (parallel A) B) lamination). B) Join– split–join mixer (serial lamination ). C) Lshape passive micromixer for mixing with chaotic advection. D) Zig-zagD) C) shaped planar Active mixers take advantage of some kind of power source or mobile parts to channel (chaotic advection).15-16. induce a disturbance in the flow. Therefore, these mixers can be classified by the type of external disturber such as pressure or temperature, among others. 16 Active mixers are usually very efficient. Nevertheless, their use involves complex setups and external power sources, which difficult their implementation. Conversely, passive mixers do not require any external power source, since they are based on the use of different geometries to achieve the mixture of reagents. On the one hand, they can increase the contact surface between the two phases or reagents to mix and decrease the diffusion path between them, which improves molecular diffusion, such as in case of parallel and serial lamination (Figure 1.2 A and B). On the other hand, passive micromixers can promote chaotic advection by manipulating the laminar ﬂow in microchannels through special geometries, which short the diffusion path and thus improves mixing (Figure 1.2 C and D). Another alternative to reduce the mixing path is to form droplets of the mixed liquids, where the movement of the droplet causes an internal ﬂow and 17-18 achieves mixing inside the droplet. Micromixers based on chaotic advection with three-dimensional structures are probably the more efficient passive mixers, stable in operation and easily integrated in complex systems. Therefore, they are often used for µ-TAS developments.. Nguyen, N.-T.; Wu, Z.; J. Micromech. Microeng., 2005, 15, R1. Mansur, E.A.; Mingxing, Y.E.; Yundong, W.; Youyuan, D.; Chinese J. Chem. Eng., 2008, 16(4), 503. 16 Petersson, F.; Nilsson, A.; Jonsson, H.; Laurell, T.; Anal. Chem., 2005, 77, 1216. 17 Aref, H.; Phys. Fluids, 2002, 14, 1315. 18 Dertinger, S.K.W.; Chiu, D.T.; Jeon, N.L.; Whitesides, G.M.; Anal. Chem., 2001, 73, 1240. 14 15.
(38) 6. 1 Introduction. Figure 1.3: Schematic view of hydrodynamic focusing in a fourchannel intersection.20. A mixing technique related to parallel lamination is the so called hydrodynamic focusing. The most common configuration is a 3-inlet microchannels device, where the middle inlet is left for one flow (e.g. sample flow) while the side streams (solvent flow) work as sheath flows, reshaping the central one downstream (Figure 1.3). 19 In this way, Stream the mixing path is reduced, since a very flow thin width central stream can be achieved. Sample Moreover, the focused sheet can be flow deformed and moved out of the symmetry plane by changing flow rates of the side streams. This technique has been widely used in microfluidic applications to reduce Stream mixing time. flow. 1.1.2 INTEGRATING OPERATIONS OF THE ANALYTICAL PROCESS IN MICROSYSTEMS The development of µ-TAS entails the miniaturization and integration of sampling, transport, treatment, separation, reaction, detection and signal treatment and interpretation into a microfluidic platform. 20 Therefore, they should ideally incorporate microsensors, electronic components for the control and acquisition of signals, and microactuators for temperature or flow rate variations. Although the development of µ-TAS entails the miniaturization and integration of a complete analytical procedure and their required components, it is usual to find hybrid devices, since the miniaturization of some elements such as pumps or valves for the management of fluids, or some pre-treatment components and detection systems is still a challenge. 21 Sample pre-treatment and detection systems are important operations to incorporate. The firsts include all the steps required for enabling the adaptation of the sample to the selected analytical method; while the seconds allows the determination of the desired analyte in the sample.. 184.108.40.206 SAMPLE PRE-TREATMENT Sample pre-treatment, namely derivatization, analyte separation and preconcentration, have been integrated in microfluidic platforms.. 19 Dziubinski, M.; in: Hydrodynamic Focusing in Microfluidic Devices, Advances in Microfluidics; Dr. Ryan Kelly (Ed.), 2012, ISBN: 978-953-51-0106-2, InTech. 20 Martínez-Cisneros, C.S.; Microsistemas analíticos basados en la tecnología LTCC. Tesis Doctoral, UAB, Bellaterra, España, 2010. 21 Suzuki, H.; Yoneyama, R.; Sens. Actuators, B, 2003, 96, 38..
(39) 1 Introduction. Derivatization operations such as labelling or complexation are performed by the use of auxiliary channels connecting the sample into specific areas, structures or mixers previous to analyte detection. 22 On the other hand, the introduction of separation techniques in microfluidic systems has provide great advantages, since these approaches allow increasing sensitivity by pre-concentration of the sample or the selectivity by eliminating interferences from the matrix. With this aim, the introduction of adsorbent materials for solid phase extraction inside microfluidic structures has been used, despite the fact that the pre-concentration area/zone is often filled after the fabrication of the microfluidic platform. 23 Other approaches such as filtration, or precipitation can be also used to eliminate interferences of the sample. Other sample pre-treatment procedures consist on heating or cooling. As well heating/cooling as temperature control has been integrated into microfluidic platforms. Some approaches are based on air or liquid cycles, 24 or integrated resistances fabricated by screen-printed techniques, which usually involve electronic instrumentation. 25 Regarding sensors for temperature control, examples of thermocouples or embedded thermistors can be also found in the literature. 26 In these fields, a monolithic integration of the thermoactuator and the microfluidic platform is usually preferred, because it confers better temperature control than modular approaches.. 220.127.116.11 DETECTION SYSTEMS Detection systems are responsible for identification and quantification of the analyte. The Group of Sensors and Biosensors (GSB) has a wealth of experience in the development of different microfluidic devices incorporating electrochemical (potentiometric 27 and voltammetric 28) and optical (absorbance, 29 fluorescence 30 and chemioluminiscence 31 ) detection systems. Electrochemical methods are easily integrated in microfluidic systems and provide high sensitivity. However, 22. Chen , D.; Mauk, M.; Qiu, X.; Liu, C.; Kim, J.; Ramprasad, S.; Ongagna, S.; Abrams, W.R.; Malamud, D.; Corstjens, P.L.A.M.; Bau, H.H.; Biomed. Microdevices, 2010, 12, 705. 23 Fang, Z.L.; in: Flow-Injection Separation and Preconcentration; VCH, Weinheim, 1993. 24 Wittwer, C.T.; Garling, D.J.; BioTechniques, 1991, 10, 76. 25 Hsueh, Y. -T; Smith, R. L; Northrup, M. A; Proc. 8th Int. Conf. Solid State Sensors Actuators (Transducers ’95), 1995, 768. 26 Liu, J.; Lu, Y.; J. Am. Chem. Soc., 2003, 125, 6642. 27 Martinez-Cisneros, C.S.; Ibañez-García, N.; Valdés, F.; Alonso, J.; Anal. Chem., 2007, 79(21), 8376. 28 Martínez-Cisneros, S.C.; Da Rocha, Z.M.; Ferreira, M.; Valdés F.; Seabra, A.; Góngora-Rubio, M.; Alonso, J.; Anal. Chem., 2009, 81, 7448. 29 Puyol, M.; Villuendas, F.; Domínguez, C.; Cadarso, V.; Llobera, A.; Salinas, I.; Garcés, I.; Alonso, J.; in: Absorbance-based integrated optical sensors; Springer Series on Chemical Sensors and Biosensors. Vol. 3 Frontiers in Optical Sensing: Novel Principles and Techniques, Ed. Springer-Verlag Berlin Heidelberg, 2005, 1-44. 30 Rivera, L.; Izquierdo, D.; Garcés, I.; Salinas, I.; Alonso, J.; Puyol, M.; Sens. Actuators, B, 2009, 137, 2, 420. 31 Ibanez-Garcia, N.; Puyol, M.; Azevedo, C. M.; Martinez-Cisneros, C. S.; Villuendas, F.; GongoraRubio, M. R.; Seabra, A. C.; Alonso, J.; Anal. Chem., 2008, 80, 14, 5320.. 7.
(40) 8. 1 Introduction. bulky instruments must be connected to the integrated electrodes, which hinders the main idea of miniaturization, and usually present electrical interferences. Optical methods are usually simpler, easier to implement in microsystems and, especially fluorescence, highly sensitive. They are very common in classical chemical methods, and a large number of reference methods are based on optical measurements. Indirect measurements based on the use of optical labels or indicators to detect and quantify the analyte are the preferred strategies and it is even possible to perform multiparameter analysis when different labels are used in the same analysis. Fluorescent labels are of special interest due to the high sensitivity of the technique and the possibility to improve selectivity, since one can discriminate between two wavelengths (excitation/emission). Moreover, few molecules show fluorescence, which considerably reduces any possible matrix interference. The components of an optical system are basically a radiation source capable of emitting a beam of light at the wavelength where the analyte or even the label absorb (in case of polychromatic light sources, wavelength selectors are required), and a detector capable to detect the changes in the signal derived from the interaction of the analyte/label and radiation. In case of fluorescence, optical filters are also required in order to eliminate light from the excitation source and thus enhance fluorescence sensitivity. Due to the advances in optoelectronics, it is easy to find cheap commercial miniaturized optical components such as LEDs, laser diodes, photodiodes, filters or phototransistors, a fact that allowed the implementation of optical systems in µ-TAS. Although laser diodes offer the possibility of working in a range from the ultraviolet to far infrared, LEDs, which emit from the visible to the medium infrared spectrum, are more commonly used due to their lower price and robustness. Photodiodes are the usual detectors integrated in µ-TAS, 32-33 since they are simpler and cheaper than phototransistors, photoresistors or photomultipliers. Despite all these features, certain limitations appear when miniaturizing optical systems. Sensitivity is compromised due to the reduction of the optical path lengths, which sometimes must be taken into account when designing optical cells in the microsystem, and more sensitive detectors as photomultipliers are required. Other limitations are related to sample matrix because turbidity can disturb the transmitted light. This issue can be overcome by coupling a simple turbidity measurement system with another light source employed as a signal reference.. 32 33. O’Toole, M.; Diamond, D.; Sensors, 2008, 2453. Rocha, F.R.P.; Reis, B.F.; Anal. Chim. Acta, 2000, 409(1-2), 227..
(41) 1 Introduction. 1.1.3 MATERIALS AND MICROFABRICATION METHODS The proper selection of the microfluidic platform substrate is crucial in order to integrate all the required operations, and it is closely related to its final application. In this sense, some characteristics such us the possibility of integrating electronic components, the intrinsic properties of the materials (transparency, chemical stability, biocompatibility, flexibility or roughness), and prototyping simplicity must be taken into account. Besides, other considerations for their future market launch such as cost and mass production possibility are to be assessed. An overview of the most commonly used materials and associated technologies is given in the future section.. 18.104.22.168 SILICON TECHNOLOGY As it can be observed for the number of publications, silicon is the most commonly used material for µ-TAS or Lab-on-a-Chip development. This responds to the well established associated technology and the extensive knowledge of its physical and chemical properties. 34-35 Silicon has also gained importance in the miniaturization field, since it is an economic and abundant material that can be obtained and processed in a controlled way. Moreover, it permits the integration of electronic components and imprinted patterns, and very complex small structures can be accurately fabricated in mass. Silicon mechanization can be performed in surface or volume through different processes, such as photolithography, wet and dry etching. In surface mechanization elements are defined on layers deposited or grown on the substrate with the aid of sacrificial layers. In volume micromachining cavities are defined within the silicon wafer, sometimes crossing the entire wafer. In some cases it is necessary the sealing of the different mechanized silicon wafers, which can be performed by anodic bonding with glass, pressure 36 or adhesive layers. 37 Figure 1.4 shows an example of a microfluidic silicon/glass device constructed with the described technology. Silicon technology requires the use of clean rooms and skilled professionals, and becomes a costly technique for prototyping purposes and therefore, it presents important limitations for research. However, silicon technology is widespread in the microelectronic field, since it is the material substrate for integrated electronic circuits and has been used in the development of passive electronic components, 38 microfluidic systems 39 or Micro Electro Mechanical Systems Bustillo, J.M.; Howe, R.T.; Muller, R.S.; Proc. IEEE, 1998, 86, 1552. Kovacs, G.T.A.; Maluf, N.I.; Petersen, K.E.; Proc IEEE, 1998, 86, 1536. 36 Gong, S.C.; Sens. Mater., 2004, 16(3), 119. 37 Kim, J.-M.; Oh, D.H.; Yoon, J.; Cho, S.; Kim, N.; Cho, J.; Kwon, Y.; Cheon, C.; Kim, Y.-K.; J. Micromech. Microeng., 2005, 15(11), N11. 38 Zhang, J.; Hon, W.C.; Leung, L.L.W.; Chen, K.J.; J. Micromech. Microeng., 2005, 15, 328. 34 35. 9.
(42) 10. 1 Introduction. (MEMS). 40 Other silicon based devices are integrated optic systems, which are composed of all silicon-made refractive lenses, optical waveguides and diodes attached to polymeric or glass microfluidic platforms. 41. Figure 1.4: Glass-silicon chip, from Micronit.. 22.214.171.124 POLYMERS TECHNOLOGY The use of polymers has increased in recent years due to their low cost and their associated simple fabrication processes, which enable prototyping in shorter time than silicon. Polymers are macromolecular substances consisting of more than 1000 repeated structural units (monomers) synthesized through a process of polymerization, which is induced by initiators or an external physical parameter. In this process, the glass transition temperature (Tg) of the material plays an important role, since it enables its structuring by solidifying or becoming softer below or above this temperature. Polymers usually contain other compounds, such as filling elements (mica, talc, calcium carbonate), plasticizers, or temperature or UV radiation stabilizers. Thus, the derived diverse polymeric compounds, commonly called plastics, exhibit different optical, chemical and thermal properties. One of the possible classifications of polymers depending on how they are linked (chemical bonds or intermolecular forces) and on the arrangement of the different chains that forms the polymer is themoplastics, elastomerics or duroplastics. 42 The firsts consist of chains of weakly attached molecules that can be modelled at temperatures above their Tg before they are cooled again. Elastomeric polymers are composed of weakly cross linked chains, and can be deformed using an external force and coming back to its initial state. Finally, duroplastic polymers are composed of strongly cross linked chains, which results in hard and fragile materials. The selection of the polymeric material to be employed for µ-TAS development will mainly depend on the chemical resistivity of the polymer, as well as its biocompatibility and transparency. Pal, P.; Sato, K.; J. Micromech. Microeng., 2009, 19, 1. Wang, F.; Li, X.X.; Guo, N.X.; Wang, Y.L.; Feng, S.L.; J. Micromech. Microeng., 2006, 16(7), 1215. 41 Cleary, A.; Glidle, A.; Laybourn, P.J.R.; Appl. Phys. Lett., 2007, 91, 071123. 42 Becker, H.; Gartner, C.; Electrophoresis, 2000, 21(1), 12. 39 40.
(43) 1 Introduction. Polymeric platforms can be fabricated by diverse techniques, which include hot embossing, 43 injection molding, 44 laser photoablation 45 and soft lithography, 46 among others, for pattering the substrate. Once the substrate is mechanized, the different polymeric layers are linked by lamination, 47 thermo-compression, 48 laser welding, 49 plasma oxidation 50 or by means of adhesives. 51 Since the fabrication technology is based on a multilayer approach, one of the main advantages of these materials is the simple fabrication of complex structures, such as three-dimensional micromixers. Figure 1.5 shows an example of a microfluidic platform based on COC polymeric substrate. Nevertheless, delamination of the layers is still a handicap in order to avoid liquid leakage. Moreover, the difficult integration of electronic components limits the use of these materials in some applications such as the development of electrochemical devices. Figure 1.5: Plastic microfluidic chip, from Microflexis.. . CYCLIC OLEFIN COPOLYMER (COC) Cyclic Olefin Copolymer (COC) consists of amorphous, transparent copolymers based on cyclic and linear olefins. It is a thermoplastic material that exhibits a unique combination of properties, which can be customized by the modification of the chemical structure of the copolymer. Performance benefits include low density, high transparency, variable heat deflection temperature up to 170 °C, excellent biocompatibility, good resistance to acid and alkali, good electrical insulating properties, good melt processability/flowability, and high rigidity, Soper, S.A.; Ford, S.M.; Qi, S.; McCarley, R.L.; Kelly, K.; Murphy, M.C.; Anal. Chem., 2000, 72, 624. Mekaru, H.; Yamada, T.; Yan, S.; Hattori, T.; Microsyst. Technol., 2004, 10, 682. 45 Nayak, N.C.; Lam, Y.C.; Yue, C.Y.; Sinha, A.T.; J. Micromech. Microeng., 2008, 18, 1. 46 McDonald, J.C.; Duffy, D.C.; Anderson, J.R.; Chiu, D.T.: Wu. H.; Schueller, O.J.; Whitesides, G.M.; Electrophoresis, 2000, 21, 27. 47 Soane, D.S.; Soane, Z.M.; Hooper, H.H.; Alonso-Amigo, M.G.; International Patent Application WO 98/45693. 48 Paulus, A.; Williams, S.J.; Sassi, A.P.; Kao, P.H.; Tan, H.; Hooper, H.H.; Proc. SPIE 3515, Microfluidic Devices and Systems, 1998, 94, 3515. 49 Malek, C.G.K.; Anal. Bioanal Chem., 2006, 185, 1362. 50 Duffy, D.C.; McDonald, J.C.; Schueller, O.J.A.; Whitesides, G.M.; Anal. Chem., 1998, 70, 4974. 51 Chen, H.Y.; McClelland, A.A.; Chen, Z.; Lahann, J.; Anal. Chem., 2008, 80, 4119. 43 44. 11.
(44) 12. 1 Introduction. strength and hardness. All this enables the construction of microfluidic platforms for multiple possible applications. The fact that one can find different COC polymerization degrees offers the possibility of working with materials/layers of different glass transition temperatures (Tg) according to the grade of the product, which simplifies the lamination process. One of the problems related to the construction of µ-TAS with polymers is the obstruction of the microfluidic structures during the sealing process. With COC, some layers of lower Tg can be used as sealing layers while others keep their structure during the lamination process. Therefore, no occlusion of deformation of the microstructures occur. However, the monolithic integration of electronic components is still a limitation for this material, since this entails a considerable complex design, high cost and a long time fabrication process. Therefore, most of the presented works are based on modular or hybrid systems as an alternative, where the different necessary components are not integrated in a single device. 52-53. 126.96.36.199 LTCC TECHNOLOGY The LTCC (Low Temperature Co-fired Ceramics) technology was originally developed by Hughes and DuPont with military purposes, and it was conceived as a hybrid sharing the advantages of thick film and High Temperature Co-fired Ceramics (HTCC) technologies. The term "low temperature" is related with the low temperatures required for the sintering process, which takes place at temperatures below 1000 °C; whereas "co-fired" refers to the possibility of sintering together screen-printing conductor pastes and the ceramic substrate, since both compounds are completely compatible. From here it follows that the technology enables the integration of other key elements, reducing significantly the total costs of the process. The LTCC ceramics can be also called as green tapes, since the substrate is manipulated in its green state, when it is malleable and soft. Once sintered, the material turns hard. This is due to their chemical composition, which include a 45 % of alumina (Al 2 O 3 ), a 40 % of silica (SiO 2 ) and a 15 % of organic components. These last organic compounds include plasticizers, which provides flexibility to the layers; an agglutinative agent or binder, which fix the ceramic particles; and solvents, which helps to solvate all the different organic additives, provides an adequate viscosity and aids to disperse the ceramic particles. 54 The LTCC technology is compatible with screen-printing techniques (thick-film technology), allowing the deposition of conductive pastes, which makes feasible the integration of electronic components. However, the pastes must be Becker, H.; Locascio, L.E.; Talanta, 2002, 56(2), 267. Pfohl, T.; Mugele, F.; Seemann, R.; Herminghaus, S.; Chem. Phys. Chem., 2003, 4(12), 1291. 54 Luo, X.J.; Zhang, B.L.; Li1, W.L.; Zhuang, H.R.; J. Mater. Sci., 2004, 39, 4387. 52 53.
(45) 1 Introduction. compatible with the sintering process. The technology is simple, does not require the use of clean rooms or specific personnel, and the implementation of mass production at low costs is feasible. Ceramic devices are fabricated by using a multilayer approach. During the procedure, the different LTCC layers are mechanized, conductive tracks are screen-printed into the necessary layers, and a lamination process is done before sintering the ceramic block. Is in this last step, where silica particles are melted and surrounds the alumina particles by capillarity, resulting in a rigid structure when the device is cooled to room temperature due to glass vitrification. In this process, the ceramic substrate suffers shrinkage. However, following the datasheets provided by the different suppliers this shrinkage is easily predictable and must be taken into account in the designing step. Then, the technology and its associated materials appear as an alternative methodology for the construction of devices with chemical purposes, providing the possibility of integrating different steps of the analytical process, such as the sample preparation, detection systems (photometric, potentiometric or voltamperometric, among others), pretreatment steps (such as mixers, gas diffusers or preconcentration chambers) and microactuators for flow control (micropumps or microvalves). 55 In this sense, GSB is a pioneer in the development of microfluidic structures with this substrate, which has given rise to many different analytical microsystems.27-28,31 Autonomous devices can be feasible obtained, which could detect different analytes as well as acquire and process the received signals. An example of a ceramic µ-TAS is presented in figure 1.6, where fluidics and electronics have been monolithically integrated in a single Figure 1.6: device.27. Gongora-Rubio, M.; Sola-Laguna, L.M.; Moffett, P.J.; Santiago Aviles, J.J.; Sens. Actuators, A, 1999, 73, 215. 55. 13. Ceramic microfluidic chip for potentiometric measurements, which integrates the fluidics and electronics in a single device. A) Bottom view of the monolithic with the electronics for data acquisition and digital signal processing. B) Top view of the microanalyzer. Fluidics and the detection system are integrated on this side. C) Lateral view of the device. 27.
(46) 14. 1 Introduction. 1.2 NANOTECHNOLGY AND ANALYTICAL CHEMISTRY Nanotechnology has emerged in recent years as a key development technology in different fields, where it has decisive economic, ecological and social impact. Its most accepted definition is the understanding and development of matter at nanoscale. This involves not only the study, design, synthesis, manipulation and application of nanomaterials, apparatus and functional systems; but also taking advantage of the physicochemical properties of nanomaterials at the nanoscale.7,56 The term nano refers to the size, and comes from the Greek word nanos, which means dwarf, and designates a billionth fraction of a unit. Nanosize generally deals from 1 to 100 nanometers (Figure 1.7). Therefore, nanotechnology studies materials, which are between atoms or molecules and bulk materials. Figure 1.7: Comparing scale from meter to nanometer dimensions.. Cat (0.3 m). Bee (15 mm) Head of a pin (1 mm). Microelectromechanical devices (10-100 µm). E. coli bacterium (~2 µm long). DNA (2 nm wide). 10 0 m. 1 meter (m). 10 - 1 m. 0.1 m 100 mm. 10 - 2 m. 0.01 m 1 cm 10 mm. 10 - 3 m. 1 mm. 10 - 4 m. 0.1 mm 100 µm. 10 - 5 m. 0.01 mm 10 µm. 10 - 6 m. 1 µm. 10 - 7 m. 0.1 µm 100 nm. 10 - 8 m. 0.01 µm 10 nm. 10 - 9 m. 1 nm. 10 - 10 m. Butterfly (0.1 m) Ant (5 mm) Dust Mite (300 µm). Human hair (50 µm) Red blood cells (2.5 µm) Hemoglobin (5.5 nm) Carbon nanotube (2 nm diameter). 0.1 nm. Althougth nanotechnology has begun to be a “well-known” technology at the end of the XX century, it has been widely used by ancient civilizations unconsciously to create beautiful and increadible materials. One of the first examples is the Lycurgus cup (Figure 1.8), from the 4th century before Christ, a Roman glass cage cup made of a dichroic glass, which makes use of small gold nanoparticles to create luminous green pigments when light comes from the front (reflected light),. 56. Ratner, M.; Ratner, D.; in: Nanotechnology: A Gentle Introduction to the Next Big Idea; Prentice Hall PTR 1st edition, 2003..
(47) 1 Introduction. whereas displays red when light comes from inside the cup (transmitted light). 57 Nanotechnology was also used by artisans in Mesopotamia (9th century) in order to generate a glittering effect on the surface of pots by the presence of cupper and silver nanoparticles on its surface. 58 In the medieval age, the artists changed the composition of the materials to create colors in the stained glass windows of churches. The study of this glasses revealed the existance of silver and gold 59-60 nanoparticles. As we have seen, the use of particles at nanosize was an usual methodology for the pigmentation of objects, but it was not until 1857 that the first scientific evaluation of nanoparticles took place, when Michael Faraday prepared the first pure sample of gold colloid (called “activated gold”) and stated that the red colour was due to the small size of these particles. 61 Other more recent approaches involving technology at nanoscale are the development of powerful electron microscopes or in the industrial field the development of branching polymers and combinatorial chemistry. But it was not until the middle of the XX century, when all this works were included in the field of nanotechnology. Ideas and concepts behind nanotechnology were firstly pointed out by the physicist Richard Feynman, which is today considered the father of the nanotechnology. On December 29th, 1959, Feynman gave a lecture in one of the American Physical Society meetings at the California Institute of Technology (CalTech), which he entiteled “Why cannot we write the entire 24 volumes of the Encyclopaedia Brittanica on the head of a pin?”. 62 There, he exposed the possibility of manipulating and controlling individual atoms and molecules as a highly powerful tool for synthetic chemistry. 63 However, it was not until 22 years later, with the development of the scanning tunneling microscope, that individual atoms could be observed, ginving rise to the development of nanotechnology. The importance of this technology arises in that, at nanoscale, the properties of matter show new physical or chemical effects, completely different from those Min’ko, N.I.; Nartsev, V.M.; Glass Ceram., 2008, 65(5-6), 148. Padovani, S.; Sada, C.; Mazzoldi,P.; Brunetti, B.; Borgia, I.; A. Sgamellotti,A.; Giulivi, A.; D’Acapito, F.; Battaglin, G.; J. Appl. Phys., 2003, 93, 10058. 59 Vilarigues, M.; da Silva, R.C.; Appl. Phys. A, 2004, 79(2), 373. 60 Vilarigues, M.; Fernandes, P.; Alves, L.C.; da Silva, R.C.; Nucl. Instrum Meth. B, 2009, 267(12-13), 2260. 61 Faraday, M.; Philos. Trans. R. Soc. London, 1857, 147, 145. 62 Feynmann, R. P.; Eng. Sci., 1960, 23, 22. 63 Edwards, S.A.; in: The Nanotech Pioneers. Where Are They Talking Us?; WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim, 1st edition, 2006. 57 58. 15. Figure 1.8: The Lycurgus Cup in reflected light (on the left) and in transmitted light (on the right). British Museum.65.
(48) 16. 1 Introduction. compared to atoms or molecules and their bulk material. As a consequence, many researchers are focusing their investigations on this “new” technology in order to develop novel materials with unique and unusual properties. However, it has to be highlighted that the fabrication of nanomaterials requires a multidisciplinary effort, since it is necessary to understand what is happening at this scale for developing useful materials. 64 In the last 20 years, huge advances have been done towards the understanding and control of matter at nanoscale. This has generated not only thousands of publications and patents in different fields, but also the development of companies with new or improved products, involving the use of nanomaterials. One can find lots of products in the market, including antibacterial socks, baseball bats with better flex and "kick", stiffer tennis rackets, wrinkle- and stain-resistant clothing, deep-penetrating therapeutic cosmetics, clear sunscreens, scratch-resistant glass coatings, faster-recharging batteries for cordless electric tools, and improved displays for televisions, cell phones, and digital cameras. 65 A large amount of nanostructured compounds or materials in the nature exist, which researchers are beginning to locate, isolate, characterize and classify. The main characteristic of these materials is that they present no human modification or processing and show remarkable properties inherent to their nanostructures. An example can be the self-cleaning property of the lotus plant, which is the combination of the microstructure of the leaves and of the epidermal cells on its rough surface, which are covered with wax crystals (Figure 1.9). 66 Other example could be the large water-repellent force of water striders, which is produced by nanostructures on its leg. Besides the self-cleaning and water-repellent force properties, many other extraordinary characteristics such as high adhesion, high mechanical strength, biological self-assembly, antireﬂection, structural coloration or thermal insulation properties have been observed, which scientist are trying to mimic in the lab to develop new nanomaterials and nanodevices due to their commercial interests. 67 Nanomaterials can be also manufactured and used at small scale, which normally include two main categories: fullerenes and nanoparticles. Fullerenes are molecules completely composed of carbon sheets, similar in structure to graphite, rolled in the form of hollow sphere, ellipsoid, tube, etc. Different types of fullerenes exist depending on their structural variations, such as buckyball clusters (from C 20 to C 60 compounds), linked "ball-and-chain". Borisenko, V.E.; Ossicini, S.; in: What is What in the Nanoworld A Handbook on Nanoscience and Nanotechnology; WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim, 2008. 65 http://nano.gov/timeline. [looked up on November 2013] 66 Zhang, J.; Wang, J.; Zhao, Y.; Xu, L.; Gao, X.; Zheng, Y.; Jiang, L.; Soft. Matter., 2008, 4, 2232. 67 Bhushan, B.; Phil. Trans. R. Soc. A, 2009, 367, 1445. 64.
(49) 1 Introduction. 17. Figure 1.9: Photograph (left) and SEM images (right) from the lotus plant.67. dimmers or fullerene rings, among others. 68- 69 However, ones of the most relevant types of fullerenes are carbon nanotubes (CNTs) due to their special properties. Whereas buckyball clusters are spherical in shape, nanotubes are cylindrical, with at least one end capped with a hemisphere of the buckyball structure. Although their length can be of several microns, their diameter is of few nanometers (from <1 nm up to 50 nm). 70-71 CNTs can have different structures depending on their thickness, length, type of helicity and number of layers, determining these parameters their final properties. Depending on the number of layers one can find single-wall nanotubes (SWNTs), multi-wall nanotubes (MWNTs) or double-wall nanotubes (DWNTs). The interest of CNTs resides in the combination of stiffness, strength, and tenacity observed by this material, since most of other commonly used compounds or materials present limitations in some of the presented properties. Moreover, this allotropic form of carbon presents comparable electrical and thermal conductivity to other conductive materials. 72 CNTs can be used for a wide range of applications such as in micro- and nano-electronics, technical textiles, conductive plastic, or in structural composite materials and chemical sensing, among others. Of special interest is their use as analytical tools due to their unique properties. 73 CNTs have been satisfactory used as column packing material for gas chromatography, 74 and as pseudo-stationary phases in capillary electrophoresis for electrolyte separation. 75 On the other hand, this nanostructured material can be also used in analyte preconcentration steps or as sorbent packed materials. In this sense, CNTs have demonstrated their suitability for the elimination of hydrocarbons from petroleum 76 and also for pre-concentrate rare earth and trace Prato, M.; J. Mater. Chem., 1997, 7(7), 1097. Bosi, S.; Da Ros, T.; Spalluto, G.; Prato, M.; Eur. J. Med. Chem., 2003, 38, 913. 70 Rao, C.N.R.; Satishkumar, B.C.; Govindaraj, A.; Nath, M.; Chem. Phys. Chem., 2001, 2, 78. 71 Endo, M; Strano, M.; Ajayan, P.; in: Carbon nanotubes; Springer Berlin, Heildelberg, 2008, 111, 13. 72 Saito, R.; Dresselhaus, G.; Dresselhaus, M.S.; in: Physical properties of carbon nanotubes; Imperial College Press, London, 1998. 73 Valcárcel, M.; Simonet, B.M.; Cárdenas, S.; Suárez, B.; Anal. Bioanal. Chem., 2005, 382, 1783. 74 Li, Q.L.; Yuan, D.X.; J. Chromatogr. A, 2003, 1003, 203. 75 Wang, Z.; Luo, G.; Chen, J.; Xiao, S.; Wang, Y.; Electrophoresis, 2003, 24, 4181. 76 Long, R.Q.; Yang, R.T.; J. Am. Chem. Soc., 2001, 123, 2058. 68 69.
(50) 18. 1 Introduction. amounts of other metals. 77-78 On the other hand, CNTs have been widely used as substrates and transducer in sensors, and more concretely in electrochemical biosensors, since CNTs can promote electron-transfer reactions. The high conductivity of this nanostructured material and the possibility of modifying its surface allow their application in high sensitive and selective devices, 79 such as in the development of amperometric or voltamperometric sensors for DNA hybridization or uric acid detection. 80-81 On the other hand, nanoparticles are another type of nanostructured material with exceptional properties. Their properties and applications are described next.. 1.2.1 NANOPARTICLES AND ITS ROLE IN ANALYTICAL CHEMISTRY Nanoparticles are commonly defined as particles which have one or more dimensions in the nanoscale order (between 1 and 100 nm), and what makes them so interesting is that these nanomaterials show different properties than the particles in the bulk size, even though they have the same chemical composition. Nanoparticles can be made of a wide range of materials, such as metals, metal oxides, silicates, non-oxide ceramics, polymers, organics, carbon and biomolecules; and can be found as spheres, cylinders, platelets, tubes, etc. As in Figure 1.10 can be observed, there exist a wide range of shapes and materials, but also different dispersion media, dispersion states and surface modifications. 82 Nanoparticles exhibit some properties due to their size that makes them very interesting for their study and application. 83-84 Materials usually have the same physical and chemical properties independently of their size, while a sizedependent effect is observed at nanoscale due to quantum effects. Thus, properties like electrical conductivity, magnetic permeability, redox potential or fluorescence can be tuned depending on the size of the particle. For instance, cadmium selenide (CdSe) nanocrystals can emit fluorescence at different wavelengths depending on their size, being feasible to synthesize nanoparticles with optical properties in all the UV-Vis spectra for their use in optoelectronics as emitters or in (bio)chemical sensing as labels. 85 Moreover, these nanomaterials can act as nanoantennas, consuming very low energy. 86-87 Thus, nanoparticles with optical properties can be crucial in developing novel technologies for the Liang, P.; Liu, Y.; Guo, L.; Spectrochim. Acta, Part B, 2005, 60, 125. Liang, P.; Liu, Y.; Guo, L.; Zeng, J.; Lu, H.; J. Anal. At. Spectrom. 2004, 19, 1489. 79 Zhang, M.G.; Smith, A.; Gorski, W.; Anal. Chem, 2004, 76, 5045. 80 Wang, Z.H.; Wang, Y.M.; Luo, G.A.; Analyst, 2002, 127, 1353. 81 Cai, H.; Jiang, X.N.; He, P.A.; Fang, Y.Z.; Anal. Bioanal. Chem., 2003, 375, 287. 82 Nagarajan, R.; Hatton, T.A.; in: Nanoparticles: synthesis, stabilization, Passivation and Functionalization, American Chemical Society, 1st edition, 2008. 83 Plieth, W.J.; J. Phys. Chem., 1982, 86(16), 3166. 84 Fendler J.H.; in: Nanoparticles and Nanostructured Films, Wiley-VCH, Weinheim, 1998. 85 Mansur, H.S.; Wiley Interdiscip. Rev. Nanomed. Nanobiotechnol., 2010, 2, 113. 86 Hewageeganaa, P.; Stockman, M.I.; Infrared Phys. Technol., 2007, 50, 177. 87 Pellegrini, G.; Mattei, G.; Mazzoldi, P.; Nanotechol., 2009, 20, 065201. 77 78.